This article needs additional citations for verification. (July 2008) (Learn how and when to remove this template message)
Photographic film is a strip or sheet of transparent film base coated on one side with a gelatin emulsion containing microscopically small light-sensitive silver halide crystals. The sizes and other characteristics of the crystals determine the sensitivity, contrast, and resolution of the film.
The emulsion will gradually darken if left exposed to light, but the process is too slow and incomplete to be of any practical use. Instead, a very short exposure to the image formed by a camera lens is used to produce only a very slight chemical change, proportional to the amount of light absorbed by each crystal. This creates an invisible latent image in the emulsion, which can be chemically developed into a visible photograph. In addition to visible light, all films are sensitive to ultraviolet light, X-rays and gamma rays, and high-energy particles. Unmodified silver halide crystals are sensitive only to the blue part of the visible spectrum, producing unnatural-looking renditions of some colored subjects. This problem was resolved with the discovery that certain dyes, called sensitizing dyes, when adsorbed onto the silver halide crystals made them respond to other colors as well. First orthochromatic (sensitive to blue and green) and finally panchromatic (sensitive to all visible colors) films were developed. Panchromatic film renders all colors in shades of gray approximately matching their subjective brightness. By similar techniques, special-purpose films can be made sensitive to the infrared (IR) region of the spectrum.
In black-and-white photographic film, there is usually one layer of silver halide crystals. When the exposed silver halide grains are developed, the silver halide crystals are converted to metallic silver, which blocks light and appears as the black part of the film negative. Color film has at least three sensitive layers, incorporating different combinations of sensitizing dyes. Typically the blue-sensitive layer is on top, followed by a yellow filter layer to stop any remaining blue light from affecting the layers below. Next comes a green-and-blue sensitive layer, and a red-and-blue sensitive layer, which record the green and red images respectively. During development, the exposed silver halide crystals are converted to metallic silver, just as with black-and-white film. But in a color film, the by-products of the development reaction simultaneously combine with chemicals known as color couplers that are included either in the film itself or in the developer solution to form colored dyes. Because the by-products are created in direct proportion to the amount of exposure and development, the dye clouds formed are also in proportion to the exposure and development. Following development, the silver is converted back to silver halide crystals in the bleach step. It is removed from the film during the process of fixing the image on the film with a solution of ammonium thiosulfate or sodium thiosulfate (hypo or fixer). Fixing leaves behind only the formed color dyes, which combine to make up the colored visible image. Later color films, like Kodacolor II, have as many as 12 emulsion layers, with upwards of 20 different chemicals in each layer. Photographic film and film stock tend to be similar in composition and speed, but often not in other parameters such as frame size and length. Silver halide photographic paper is also similar to photographic film.
Characteristics of film
There are several types of photographic film, including:
- Print film, when developed, yields transparent negatives with the light and dark areas and colors (if color film is used) inverted to their respective complementary colors. This type of film is designed to be printed onto photographic paper, usually by means of an enlarger but in some cases by contact printing. The paper is then itself developed. The second inversion that results restores light, shade and color to their normal appearance. Color negatives incorporate an orange color correction mask that compensates for unwanted dye absorptions and improves color accuracy in the prints. Although color processing is more complex and temperature-sensitive than black-and-white processing, the wide availability of commercial color processing and scarcity of service for black-and-white prompted the design of some black-and-white films which are processed in exactly the same way as standard color film.
- Color reversal film produces positive transparencies, also known as diapositives. Transparencies can be reviewed with the aid of a magnifying loupe and a lightbox. If mounted in small metal, plastic or cardboard frames for use in a slide projector or slide viewer they are commonly called slides. Reversal film is often marketed as "slide film". Large-format color reversal sheet film is used by some professional photographers, typically to originate very-high-resolution imagery for digital scanning into color separations for mass photomechanical reproduction. Photographic prints can be produced from reversal film transparencies, but positive-to-positive print materials for doing this directly (e.g. Ektachrome paper, Cibachrome/Ilfochrome) have all been discontinued, so it now requires the use of an internegative to convert the positive transparency image into a negative transparency, which is then printed as a positive print.
- Black-and-white reversal film exists but is very uncommon. Conventional black-and-white negative film can be reversal-processed to produce black-and-white slides, as by dr5 Chrome. Although kits of chemicals for black-and-white reversal processing may no longer be available to amateur darkroom enthusiasts, an acid bleaching solution, the only unusual component which is essential, is easily prepared from scratch. Black-and-white transparencies may also be produced by printing negatives onto special positive print film, still available from some specialty photographic supply dealers.
In order to produce a usable image, the film needs to be exposed properly. The amount of exposure variation that a given film can tolerate, while still producing an acceptable level of quality, is called its exposure latitude. Color print film generally has greater exposure latitude than other types of film. Additionally, because print film must be printed to be viewed, after-the-fact corrections for imperfect exposure are possible during the printing process.
The concentration of dyes or silver halide crystals remaining on the film after development is referred to as optical density, or simply density; the optical density is proportional to the logarithm of the optical transmission coefficient of the developed film. A dark image on the negative is of higher density than a more transparent image.
Most films are affected by the physics of silver grain activation (which sets a minimum amount of light required to expose a single grain) and by the statistics of random grain activation by photons. The film requires a minimum amount of light before it begins to expose, and then responds by progressive darkening over a wide dynamic range of exposure until all of the grains are exposed, and the film achieves (after development) its maximum optical density.
Over the active dynamic range of most films, the density of the developed film is proportional to the logarithm of the total amount of light to which the film was exposed, so the transmission coefficient of the developed film is proportional to a power of the reciprocal of the brightness of the original exposure. The plot of the density of the film image against the log of the exposure is known as an H&D curve. This effect is due to the statistics of grain activation: as the film becomes progressively more exposed, each incident photon is less likely to impact a still-unexposed grain, yielding the logarithmic behavior. A simple, idealized statistical model yields the equation density = 1 – ( 1 – k) light, where light is proportional to the number of photons hitting a unit area of film, k is the probability of a single photon striking a grain (based on the size of the grains and how closely spaced they are), and density is the proportion of grains that have been hit by at least one photon. The relationship between density and log exposure is linear for photographic films except at the extreme ranges of maximum exposure (D-max) and minimum exposure (D-min) on an H&D curve, so the curve is characteristically S-shaped (as opposed to digital camera sensors which have a linear response through the effective exposure range). The sensitivity (i.e., the ISO speed) of a film can be affected by changing the length or temperature of development, which would move the H&D curve to the left or right (see figure).
If parts of the image are exposed heavily enough to approach the maximum density possible for a print film, then they will begin losing the ability to show tonal variations in the final print. Usually those areas will be considered overexposed and will appear as featureless white on the print. Some subject matter is tolerant of very heavy exposure. For example, sources of brilliant light, such as a light bulb or the sun, generally appear best as a featureless white on the print.
Likewise, if part of an image receives less than the beginning threshold level of exposure, which depends upon the film's sensitivity to light—or speed—the film there will have no appreciable image density, and will appear on the print as a featureless black. Some photographers use their knowledge of these limits to determine the optimum exposure for a photograph; for one example, see the Zone System. Most automatic cameras instead try to achieve a particular average density.
Color films can have many layers. The film base can have an antilahalation layer applied to it or be dyed. This layer prevents light from reflecting from within the film, increasing image quality. If applied to the back of the film, it also serves to prevent scratching, as an antistatic measure due to its conductive carbon content, and as a lubricant to help transport the film through mechanisms. The antistatic property is necessary to prevent the film from getting fogged under low humidity, and mechanisms to avoid static are present in most if not all films. If applied on the back it is removed during film processing. If applied it may be on the back of the film base in triacetate film bases or in the front in PET film bases, below the emulsion stack. An anticurl layer and a separate antistatic layer may be present in thin high resolution films that have the antihalation layer below the emulsion. PET film bases are often dyed, specially because PET can serve as a light pipe; black and white film bases tend to have a higher level of dying applied to them. The film base needs to be transparent but with some density, perfectly flat, insensitive to light, chemically stable, resistant to tearing and strong enough to be handled manually and by camera mechanisms and film processing equipment, while being chemically resistant to moisture and the chemicals used during processing without losing strength, flexibility or changing in size.
The subbing layer is essentially an adhesive that allows the subsequent layers to stick to the film base. The film base was initially made of highly flammable cellulose nitrate, which was replaced by cellulose acetate films, often cellulose triacetate film (safety film), which in turn was replaced in many films (such as all print films, most duplication films and some other specialty films) by a PET (polyethylene terephthalate) plastic film base. Films with a triacetate base can suffer from vinegar syndrome, a decomposition process that releases acetic acid under warm and humid conditions, which is the characteristic component of vinegar, imparting the film a strong vinegar smell and possibly even damaging surrounding metal and films. Films are usually spliced using a special adhesive tape; those with PET layers can be ultrasonically spliced or their ends melted and then spliced.
The emulsion layers of films are made by dissolving pure silver in nitric acid to form silver nitrate crystals, which are mixed with other chemicals to form silver halide grains, which are then suspended in gelatin and applied to the film base. The size and hence the light sensitivity of these grains determines the speed of the film; since films contain real silver (as silver halide), faster films with larger crystals are more expensive and potentially subject to variations in the price of silver metal. Also, since the grains are larger, faster films have more grain. Each crystal is often 0.2 to 2 microns in size; in color films, the dye clouds that surround the silver halide crystals are often 25 microns across. The crystals can be shaped as cubes, rectangles, tetradecadedrons, hexagons or be flat and resemble a triangle with or without clipped edges; this type of crystal is known as a T-grain crystal. Films using T-grains are more sensitive to light without using more silver halide since they increase the surface area exposed to light by making the crystals flatter and larger in footprint instead of simply increasing their size.
In color films, each emulsion layer has a different color dye forming coupler: in the blue sensitive layer, the coupler forms a yellow dye; in the green sensitive layer the coupler forms a magenta dye, and in the red sensitive layer the coupler forms a cyan dye. Color films often have an UV blocking layer. Each emulsion layer in a color film may itself have three layers: a slow, medium and fast layer, to allow the film to capture higher contrast images. The color dye couplers are inside oil droplets dispered in the emulsion around silver halide crystals, forming a silver halide grain. Here the oil droplets act as a surfactant, also protecting the couplers from chemical reactions with the silver halide and from the surrounding gelatin. During development, oxidized developer diffuses into the oil droplets and combines with the dye couplers to form dye clouds; the dye clouds only form around unexposed silver halide crystals. The fixer then removes the silver halide crystals leaving only the dye clouds: this means that developed color films may not contain silver while undeveloped films do contain silver; this also means that the fixer can start to contain silver which can then be removed through electrolysis. Color films also contain light filters to filter out certain colors as the light passes through the film: often there is a blue light filter between the blue and green sensitive layers and a yellow filter before the red sensitive layer; in this way each layer is made sensitive to only a certain color of light.
The color couplers may be colorless and be chromogenic or be colored. Colored couplers are used to improve the color reproduction of film. The first coupler which is used in the blue layer remains colorless to allow all light to pass through, but the coupler used in the green layer is colored yellow, and the coupler used in the red layer is light pink. Yellow was chosen to block any remaining blue light from exposing the underlying green and red layers (since yellow can be made from green and red). Each layer should only be sensitive to a single color of light and allow all others to pass through. Because of these colored couplers, the developed film appears orange. Colored couplers mean that corrections through color filters need to be applied to the image before printing. Printing can be carried out by using an optical enlarger, or by scanning the image, correcting it using software and printing it using a digital printer.
Kodachrome films have no couplers; the dyes are instead formed by a long sequence of steps, limiting adoption among smaller film processing companies.
Black and white films are very simple by comparison, only consisting of silver halide crystals suspended in a gelatin emulsion which sits on a film base with an antihalation back.
Many films contain a top supercoat layer to protect the emulsion layers from damage. Some manufacturers manufacture their films with daylight, tungsten (named after the tungsten filament of incandescent and halogen lamps) or fluorescent lighting in mind, recommending the use of lens filters, light meters and test shots in some situations to maintain color balance, or by recommending the division of the ISO value of the film by the distance of the subject from the camera to get an appropriate f-number value to be set in the lens.
Examples of Color films are Kodachrome, often processed using the K-14 process, Kodacolor, Ektachrome, which is often processed using the E-6 process and Fujifilm Superia, which is processed using the C-41 process. The chemicals and the color dye couplers on the film may vary depending on the process used to develop the film.
Film speed describes a film's threshold sensitivity to light. The international standard for rating film speed is the ISO#ISO scale, which combines both the ASA speed and the DIN speed in the format ASA/DIN. Using ISO convention film with an ASA speed of 400 would be labeled 400/27°. A fourth naming standard is GOST, developed by the Russian standards authority. See the film speed article for a table of conversions between ASA, DIN, and GOST film speeds.
Common film speeds include ISO 25, 50, 64, 100, 160, 200, 400, 800, 1600, 3200, and 6400. Consumer print films are usually in the ISO 100 to ISO 800 range. Some films, like Kodak's Technical Pan, are not ISO rated and therefore careful examination of the film's properties must be made by the photographer before exposure and development. ISO 25 film is very "slow", as it requires much more exposure to produce a usable image than "fast" ISO 800 film. Films of ISO 800 and greater are thus better suited to low-light situations and action shots (where the short exposure time limits the total light received). The benefit of slower film is that it usually has finer grain and better color rendition than fast film. Professional photographers of static subjects such as portraits or landscapes usually seek these qualities, and therefore require a tripod to stabilize the camera for a longer exposure. A professional photographing subjects such as rapidly moving sports or in low-light conditions will inevitably choose a faster film.
A film with a particular ISO rating can be push-processed, or "pushed", to behave like a film with a higher ISO, by developing for a longer amount of time or at a higher temperature than usual.:160 More rarely, a film can be "pulled" to behave like a "slower" film. Pushing generally coarsens grain and increases contrast, reducing dynamic range, to the detriment of overall quality. Nevertheless, it can be a useful tradeoff in difficult shooting environments, if the alternative is no usable shot at all.
Instant photography, as popularized by Polaroid, uses a special type of camera and film that automates and integrates development, without the need of further equipment or chemicals. This process is carried out immediately after exposure, as opposed to regular film, which is developed afterwards and requires additional chemicals. See instant film.
Films can be made to record non-visible ultraviolet (UV) and infrared (IR) radiation. These films generally require special equipment; for example, most photographic lenses are made of glass and will therefore filter out most ultraviolet light. Instead, expensive lenses made of quartz must be used. Infrared films may be shot in standard cameras using an infrared band- or long-pass filters, although the infrared focal point must be compensated for.
Exposure and focusing are difficult when using UV or IR film with a camera and lens designed for visible light. The ISO standard for film speed only applies to visible light, so visual-spectrum light meters are nearly useless. Film manufacturers can supply suggested equivalent film speeds under different conditions, and recommend heavy bracketing (e.g., with a certain filter, assume ISO 25 under daylight and ISO 64 under tungsten lighting). This allows a light meter to be used to estimate an exposure. The focal point for IR is slightly farther away from the camera than visible light, and UV slightly closer; this must be compensated for when focusing. Apochromatic lenses are sometimes recommended due to their improved focusing across the spectrum.
Film optimized for detecting X-ray radiation is commonly used for medical radiography and industrial radiography by placing the subject between the film and a source of X-rays or gamma rays, without a lens, as if a translucent object were imaged by being placed between a light source and standard film. Unlike other types of film, X-ray film has a sensitive emulsion on both sides of the carrier material. This reduces the X-ray exposure for an acceptable image – a desirable feature in medical radiography. The film is usually placed in close contact with phosphor screen(s) and/or thin lead-foil screen(s), the combination having a higher sensitivity to X-rays.
Film optimized for detecting X-rays and gamma rays is sometimes used for radiation dosimetry.
Film has a number of disadvantages as a scientific detector: it is difficult to calibrate for photometry, it is not re-usable, it requires careful handling (including temperature and humidity control) for best calibration, and the film must physically be returned to the laboratory and processed. Against this, photographic film can be made with a higher spatial resolution than any other type of imaging detector, and, because of its logarithmic response to light, has a wider dynamic range than most digital detectors. For example, Agfa 10E56 holographic film has a resolution of over 4,000 lines/mm—equivalent to a pixel size of 0.125 micrometers—and an active dynamic range of over five orders of magnitude in brightness, compared to typical scientific CCDs that might have pixels of about 10 micrometers and a dynamic range of 3–4 orders of magnitude.[failed verification]
Special films are used for the long exposures required by astrophotography.
Encoding of metadata
Some film cameras have the ability to read metadata from the film canister or encode metadata on film negatives.
Negative imprinting is a feature of some film cameras, in which the date, shutter speed and aperture setting are recorded on the negative directly as the film is exposed. The first known version of this process was patented in the United States in 1975, using half-silvered mirrors to direct the readout of a digital clock and mix it with the light rays coming through the main camera lens. Modern SLR cameras use an imprinter fixed to the back of the camera on the film backing plate. It uses a small LED display for illumination and optics to focus the light onto a specific part of the film. The LED display is exposed on the negative at the same time the picture is taken. Digital cameras can often encode all the information in the image file itself. The Exif format is the most commonly used format.
In the 1980s, Kodak developed DX Encoding (from Digital indeX), or DX coding, a feature that was eventually adapted by all camera and film manufacturers. DX encoding provides information on both the film cassette and on the film regarding the type of film, number of exposures, speed (ISO/ASA rating) of the film. It consists of three types of identification. First is a barcode near the film opening of the cassette, identifying the manufacturer, film type and processing method (see image below left). This is used by photofinishing equipment during film processing. The second part is a barcode on the edge of the film (see image below right), used also during processing, which indicates the image film type, manufacturer, frame number and synchronizes the position of the frame. The third part of DX coding, known as the DX Camera Auto Sensing (CAS) code, consists of a series of 12 metal contacts on the film cassette, which beginning with cameras manufactured after 1985 could detect the type of film, number of exposures and ISO of the film, and use that information to automatically adjust the camera settings for the speed of the film.
Common sizes of film
|Film Designation||Film width (mm)||Image size (mm)||Number of images||Reasons|
|110||16||13 × 17||12/20||Single perforations, cartridge loaded|
|APS/IX240||24||17 × 30||15/25/40||
e.g., Kodak "Advantix", different aspect ratios possible, data recorded on magnetic strip, processed film remains in cartridge
|126||35||26 × 26||12/20/24||Single perforations, cartridge loaded, e.g., Kodak Instamatic camera|
|135||35||24 × 36 (1.0 x 1.5 in.)||12–36||Double perforations, cassette loaded, "35 mm film"|
|127||46||40 x 40 (also 40 x 30 or 60)||8-16||Unperforated, rolled in backing paper.|
|120||62||45 × 60||16 or 15||Unperforated, rolled in backing paper. For medium format photography|
|60 × 60||12|
|60 × 70||10|
|60 × 90||8|
|220||62||45 �� 60||32 or 31||Same as 120, but rolled with no backing paper, allowing for double the number of images. Unperforated film with leader and trailer.|
|60 × 60||24|
|60 × 70||20|
|60 × 90||16|
|Sheet film||2 ¼ x 3 ¼ to 20 x 24 in.||1||Individual sheets of film, notched in corner for identification, for large format photography|
|Disc film||10 × 8 mm||15|
|Motion picture films||8 mm, 16 mm, 35 mm and 70 mm||Double perforations, cassette loaded|
History of film
The earliest practical photographic process was the daguerreotype; it was introduced in 1839 and did not use film. The light-sensitive chemicals were formed on the surface of a silver-plated copper sheet. The calotype process produced paper negatives. Beginning in the 1850s, thin glass plates coated with photographic emulsion became the standard material for use in the camera. Although fragile and relatively heavy, the glass used for photographic plates was of better optical quality than early transparent plastics and was, at first, less expensive. Glass plates continued to be used long after the introduction of film, and were used for astrophotography and electron micrography until the early 2000s, when they were supplanted by digital recording methods. Ilford continues to manufacture glass plates for special scientific applications.
The first flexible photographic roll film was sold by George Eastman in 1885, but this original "film" was actually a coating on a paper base. As part of the processing, the image-bearing layer was stripped from the paper and attached to a sheet of hardened clear gelatin. The first transparent plastic roll film followed in 1889. It was made from highly flammable cellulose nitrate film.
Although cellulose acetate or "safety film" had been introduced by Kodak in 1908, at first it found only a few special applications as an alternative to the hazardous nitrate film, which had the advantages of being considerably tougher, slightly more transparent, and cheaper. The changeover was completed for X-ray films in 1933, but although safety film was always used for 16 mm and 8 mm home movies, nitrate film remained standard for theatrical 35 mm films until it was finally discontinued in 1951.
Hurter and Driffield began pioneering work on the light sensitivity of photographic emulsions in 1876. Their work enabled the first quantitative measure of film speed to be devised. They developed H&D curves, which are specific for each film and paper. These curves plot the photographic density against the log of the exposure, to determine sensitivity or speed of the emulsion and enabling correct exposure.
This section does not cite any sources. (October 2016) (Learn how and when to remove this template message)
Early photographic plates and films were usefully sensitive only to blue, violet and ultraviolet light. As a result, the relative tonal values in a scene registered roughly as they would appear if viewed through a piece of deep blue glass. Blue skies with interesting cloud formations photographed as a white blank. Any detail visible in masses of green foliage was due mainly to the colorless surface gloss. Bright yellows and reds appeared nearly black. Most skin tones came out unnaturally dark, and uneven or freckled complexions were exaggerated. Photographers sometimes compensated by adding in skies from separate negatives that had been exposed and processed to optimize the visibility of the clouds, by manually retouching their negatives to adjust problematic tonal values, and by heavily powdering the faces of their portrait sitters.
In 1873, Hermann Wilhelm Vogel discovered that the spectral sensitivity could be extended to green and yellow light by adding very small quantities of certain dyes to the emulsion. The instability of early sensitizing dyes and their tendency to rapidly cause fogging initially confined their use to the laboratory, but in 1883 the first commercially dye-sensitized plates appeared on the market. These early products, described as isochromatic or orthochromatic depending on the manufacturer, made possible a more accurate rendering of colored subject matter into a black-and-white image. Because they were still disproportionately sensitive to blue, the use of a yellow filter and a consequently longer exposure time were required to take full advantage of their extended sensitivity.
In 1894, the Lumière Brothers introduced their Lumière Panchromatic plate, which was made sensitive, although very unequally, to all colors including red. New and improved sensitizing dyes were developed, and in 1902 the much more evenly color-sensitive Perchromo panchromatic plate was being sold by the German manufacturer Perutz. The commercial availability of highly panchromatic black-and-white emulsions also accelerated the progress of practical color photography, which requires good sensitivity to all the colors of the spectrum for the red, green and blue channels of color information to all be captured with reasonable exposure times.
However, all of these were glass-based plate products. Panchromatic emulsions on a film base were not commercially available until the 1910s and did not come into general use until much later. Many photographers who did their own darkroom work preferred to go without the seeming luxury of sensitivity to red—a rare color in nature and uncommon even in man-made objects—rather than be forced to abandon the traditional red darkroom safelight and process their exposed film in complete darkness. Kodak's popular Verichrome black-and-white snapshot film, introduced in 1931, remained a red-insensitive orthochromatic product until 1956, when it was replaced by Verichrome Pan. Amateur darkroom enthusiasts then had to handle the undeveloped film by the sense of touch alone.
Introduction to color
Experiments with color photography began almost as early as photography itself, but the three-color principle underlying all practical processes was not set forth until 1855, not demonstrated until 1861, and not generally accepted as "real" color photography until it had become an undeniable commercial reality in the early 20th century. Although color photographs of good quality were being made by the 1890s, they required special equipment, long exposures, complex printing or display procedures and highly specialized skills, so they were then exceedingly rare.
The first practical and commercially successful color "film" was the Lumière Autochrome, a glass plate product introduced in 1907. It was expensive and not sensitive enough for hand-held "snapshot" use. Film-based versions were introduced in the early 1930s and the sensitivity was later improved. These were "mosaic screen" additive color products, which used a simple layer of black-and-white emulsion in combination with a layer of microscopically small color filter elements. The resulting transparencies or "slides" were very dark because the color filter mosaic layer absorbed most of the light passing through. The last films of this type were discontinued in the 1950s, but Polachrome "instant" slide film, introduced in 1983, temporarily revived the technology.
"Color film" in the modern sense of a subtractive color product with a multi-layered emulsion was born with the introduction of Kodachrome for home movies in 1935 and as lengths of 35 mm film for still cameras in 1936; however, it required a complex development process, with multiple dyeing steps as each color layer was processed separately. 1936 also saw the launch of Agfa Color Neu, the first subtractive three-color reversal film for movie and still camera use to incorporate color dye couplers, which could be processed at the same time by a single color developer. The film had some 278 patents. The incorporation of color couplers formed the basis of subsequent color film design, with the Agfa process initially adopted by Ferrania, Fuji and Konica and lasting until the late 70s/early 1980s in the West and 1990s in Eastern Europe. The process used dye-forming chemicals that terminated with sulfonic acid groups and had to be coated one layer at a time. It was a further innovation by Kodak, using dye-forming chemicals which terminated in 'fatty' tails which permitted multiple layers to coated at the same time in a single pass, reducing production time and cost that later became universally adopted along with the Kodak C-41 process.
Despite greater availability of color film after WWII during the next several decades, it remained much more expensive than black-and-white and required much more light, factors which combined the greater cost of processing and printing delayed its widespread adoption. Decreasing cost, increasing sensitivity and standardised processing gradually overcame these impediments. By the 1970s, color film predominated in the consumer market, while the use of black-and-white film was increasingly confined to photojournalism and fine art photography.
Effect on lens and equipment design
Photographic lenses and equipment are designed around the film to be used. Although the earliest photographic materials were sensitive only to the blue-violet end of the spectrum, partially color-corrected achromatic lenses were normally used, so that when the photographer brought the visually brightest yellow rays to a sharp focus, the visually dimmest but photographically most active violet rays would be correctly focused, too. The introduction of orthochromatic emulsions required the whole range of colors from yellow to blue to be brought to an adequate focus. Most plates and films described as orthochromatic or isochromatic were practically insensitive to red, so the correct focus of red light was unimportant; a red window could be used to view the frame numbers on the paper backing of roll film, as any red light which leaked around the backing would not fog the film; and red lighting could be used in darkrooms. With the introduction of panchromatic film, the whole visible spectrum needed to be brought to an acceptably sharp focus. In all cases a color cast in the lens glass or faint colored reflections in the image were of no consequence as they would merely change the contrast a little. This was no longer acceptable when using color film. More highly corrected lenses for newer emulsions could be used with older emulsion types, but the converse was not true.
The progression of lens design for later emulsions is of practical importance when considering the use of old lenses, still often used on large-format equipment; a lens designed for orthochromatic film may have visible defects with a color emulsion; a lens for panchromatic film will be better but not as good as later designs.
The filters used were different for the different film types.
Film remained the dominant form of photography until the early 21st century, when advances in digital photography drew consumers to digital formats. The first consumer electronic camera, the Sony Mavica was released in 1981, the first digital camera, the Fuji DS-X released in 1989, coupled with advances in software such as Adobe Photoshop which was released in 1989, improvements in consumer level digital color printers and increasingly widespread computers in households during the late 20th century facilitated uptake of digital photography by consumers. Although modern photography is dominated by digital users, film continues to be used by enthusiasts. Film remains the preference of some photographers because of its distinctive "look".[a]
Renewed interest in recent years
Despite the fact that digital cameras are by far the most commonly-used photographic tool and that the selection of available photographic films is much smaller than it once was, sales of photographic film have been on a steady upward trend. Kodak (which was under bankruptcy protection from January 2012 to September 2013) and other companies have noticed this upward trend: Dennis Olbrich, President of the Imaging Paper, Photo Chemicals and Film division at Kodak Alaris, has stated that sales of their photographic films have been growing over the past 3 or 4 years. UK-based Ilford have confirmed this trend and conducted extensive research on this subject matter, their research showing that 60% of current film users had only started using film in the past five years and that 30% of current film users were under 35 years old.
In 2013 Ferrania, an Italy-based film manufacturer which ceased production of photographic films between the years 2009 and 2010, was acquired by the new Film Ferrania S.R.L taking over the old company's manufacturing facilities, and re-employed some workers who had been laid off 3 years earlier when the company stopped production of film. In November of the same year, the company started a crowdfunding campaign with the goal of raising $250,000 to buy tooling and machines from the old factory, with the intention of putting some of the films that had been discontinued back into production, the campaign succeeded and in October 2014 was ended with over $320,000 being raised.
In February 2017, Film Ferrania unveiled their "P30" 80 ASA, Panchromatic black and white film, in 35mm format.
Kodak announced on January 5, 2017, that Ektachrome, one of Kodak's most well known transparency films that had been discontinued between 2012 and 2013, would be reformulated and manufactured once again, in 35 mm still and Super 8 motion picture film formats. Following the success of the release, Kodak expanded Ektachrome's format availability by also releasing the film in 120 and 4x5 formats.
Japan-based Fujifilm's instant film "Instax" cameras and paper have also proven to be very successful, and have replaced traditional photographic films as Fujifilm's main film products, while they continue to offer traditional photographic films in various formats and types.
|ADOX||Germany||Marly, Switz||♦||♦||-||-||Commissions film manufacture and converts Agfa-Gevaert micro and aerial films for still camera use. Trial coating at Marly (former Ilford Imaging test coater).|
|Agfa-Gevaert||Belgium||Mortsel||♦||-||-||-||Business to business manufacturer of aerial and micro films|
|Bergger||France||Out-sourced||♦||-||-||-||Still film brand.|
|Cinestill||USA||Out-sourced||♦||-||♦||-||Converts Kodak movie film for still camera use.|
|FILM Ferrania||Italy||Ferrania, Liguria||♦||-||-||-||Still film using former Ferrania research coater.|
|Foma Bohemia||Czech Rep.||Hradec Králové||♦||♦||-||-||Still, movie film, X-Ray and Industrial films|
|Fujifilm||Japan||Ashigara, Tokyo||♦||-||♦||♦||Still and instant films.|
|Ilford||UK||Mobberley, Cheshire||♦||-||-||-||Major B&W still film brand owned by Harman Technology|
|Inoviscoat||Germany||Monheim am Rhein||-||-||-||-||Business to business. Still and industrial films. Established with former Agfa (Leverkusen) coater. Supplier to Polaroid.|
|Kodak||USA||Rochester, NY||♦||-||♦||♦||Still and movie films, Still film distribution by Kodak Alaris (UK)|
|Lomography||Austria||Out-sourced||♦||-||♦||♦||Brand. Films produced by Kodak and Foma Bohemia|
|Lucky||China||Baoding, Hebei province||♦||-||-||-||B&W still film|
|Micron||Russia||??||♦||-||-||-||Business-to-business scientific film manufacture owned by TD Slavich.|
|ORWO||Germany||Out-sourced||♦||-||-||-||Brand of Filmotec specialising in Movie films|
|Polaroid Originals||Netherlands||Enschede||♦*||-||♦*||-||*Instant film|
|Rollei||Germany||Out-sourced||♦||-||-||♦||Brand. Film produced by Agfa-Gevaert and Harman Technology|
|Shanghai||China||Out-sourced||♦||-||-||-||Still film and 135 film from ORWO.|
|Silberra||Russia||Out-sourced||♦||-||-||-||Brand. Still film from Agfa-Gevaert, ORWO and Micron|
|Tasma||Russia||Kazan||♦||-||-||-||Business-to-business manufacturer of aerial and industrial films|
Key: B&W – Black and white negative, B&WR – Black and white reversal, CN – Color Negative, CR- Color Reversal.
|Agfaphoto GmbH||Germany||Leverkusen||♦||♦||2004||2005||The Agfa Consumer Imaging division and its Leverkusen works was sold off by parent company Agfa-Gevaert and was insolvent within a year. Agfaphoto holdings GmbH continues as the brand owner.|
|Ansco||USA||New York||♦||♦||1850s||1980s||Part of Agfa 1928 until 1941. In later years known as GAF|
|Azumures||Romania||Târgu Mureș||♦||♦||1989||2003||Azopan/Azocolor brand.|
|efke||Croatia||Samobor||♦||-||1974||2012||Brand of Fotokemica|
|ERA||China||Shantou||♦||♦||1950||2008||Acquired by Kodak China in 1998.|
|Ferrania||Italy||Ferrania||♦||♦||1923||2009||As Ferrania-3M from 1964–1996 a major producer of 'white label' color film.|
|Fuda||China||Shanghai||♦||♦||19??||200?||Acquired by Kodak China in 1998.|
|Forte||Hungary||Vac||♦||♦*||1922||2007||*Color film was outsourced|
|Konica||Japan||??||♦||♦||1873||2006||Originally branded 'Sakura'. Major producer of 'white label' color film. Following merger with Minolta in 2003 it exited the photographic business in 2006.|
|Negra||Spain||Barcelona||♦||♦*||1928||1984||*Color film was outsourced|
|ORWO||East Germany||Wolfen||♦||♦||1945||1994||Formerly the Agfa Wolfen plant, it became VEB Film und Chemiefaserwerk post war and adopted the name ORWO in 1964. Successor company Filmotec still produces ORWO branded cine films.|
|Perutz||Germany||Munich||♦||♦||1880||1964||Acquired by Agfa 1964. Later films were rebranded Agfa material.|
|Polaroid Corporation||USA||Cambridge, Massachusetts||♦||♦||1937||2008||Instant film. Production also in Mexico, Scotland, and Netherlands.|
|Svema||Ukraine||Shostka||♦||♦||1931||2000||Brand continues under ownership of Astrum holdings.|
- List of photographic equipment makers
- List of photographic films
- Photrio (formerly APUG)
- Oversampled binary image sensor
- The distinctive "look" of film-based photographs compared to digital images is likely due to a combination of factors, including (1) differences in spectral and tonal sensitivity (S-shaped density to exposure with film, vs. linear response curve for digital CCD sensors c.f.) (2) resolution (3) continuity of tone
- Karlheinz Keller et al. "Photography" in Ullmann's Encyclopedia of Industrial Chemistry, 2005, Wiley-VCH, Weinheim. doi:10.1002/14356007.a20_001
- Rogers, David (2007). The Chemistry of Photography: From Classical to Digital Technologies. Cambridge, UK: The Royal Society of Chemistry. ISBN 978-0-85404-273-9.
- Anchell, Steve (2008). The Darkroom Cookbook p.103-105. Elsevier, Oxford OX2 8DP, UK. ISBN 978-0-240-81055-3
- Schwalberg Bob (June 1984). "Popular Photography". Popular Photography. 91 (6): 55.
- Langford, Michael (2010). Langford’s Basic Photography: The guide for serious photographers, 9th ed. Oxford, UK: Focal Press. ISBN 978-0-240-52168-8.
- "dr5CHROME B&W reversal process information". Archived from the original on 2010-08-08.
- Haist, Grant (1979). Modern photographic processing. New York: Wiley. ISBN 978-0-471-02228-2.
- Jacobson 2000, pp. 232–234.
- Peres, Michael (2007). The Focal encyclopedia of photography: digital imaging, theory and applications, history, and science (4th ed.). Burlington, MA: Focal Press. ISBN 978-0-240-80740-9.
- Peres, Michael R. (2008). The concise Focal encyclopedia of photography: from the first photo on paper to the digital revolution. Burlington, Mass.: Focal Press/Elsevier. p. 75. ISBN 978-0-240-80998-4.
- Jacobson 2000, pp. 306–309.
- "Basic Sensitometry and Characteristics of Film" (PDF). Kodak Cinema and Television: Technical Information. Kodak. Archived (PDF) from the original on 5 March 2016. Retrieved 11 August 2015.
- Ahmad, Ida R. "Historical films may be decaying much faster than we thought thanks to 'vinegar syndrome'". The Conversation.
- "Silver halide photographic emulsion and photographic material containing the same".
- "Silver halide photographic emulsion and silver halide photographic lightsensitive material using the same".
- "Captcha". www.osapublishing.org.
- "How Is Silver Bromide Used in Photography?_Chemicalbook". www.chemicalbook.com.
- "Film Structure". www2.optics.rochester.edu.
- Jacobson 2000, p. 306.
- "KODAK PROFESSIONAL Technical Pan Film Technical Data Sheet" (PDF). Eastman Kodak Company. Archived (PDF) from the original on 17 August 2000. Retrieved 13 August 2015.
- London, Barbara; Upton, John (1998). Photography (6th ed.). New York: Longman. ISBN 0-321-01108-2.
- "Archived copy". Archived from the original on 2017-12-07. Retrieved 2016-08-18.CS1 maint: archived copy as title (link)
- Malin, David; Murdin, Paul (1984-08-30). Colours of the Stars. CUP Archive. ISBN 978-0-521-25714-5.
- US 3882512, Lawrence, Franklin B. & Robert E. Lewis, "Camera system with on-frame digital recording means", published 1975-05-06
- US 8400466, Yamamoto, Shinobu, "Image retrieval apparatus, image retrieving method, and storage medium for performing the image retrieving method in the image retrieval apparatus", published 2013-03-19
- Francois (30 January 2008). "The DX story – or how the coding works". filmwasters.com. Archived from the original on 3 October 2015. Retrieved 8 August 2015.
- Grundberg, Andy (12 October 1986). "CAMERA: How to Read the Code on DX Film Cartridges". The New York Times: Arts Section. Archived from the original on 11 October 2015. Retrieved 8 August 2015.
- Jacobson 2000, p. 138.
- Jacobson 2000, pp. 200–201.
- Osterman, Mark (2007). "Technical Evolution of Photography". In Peres, Michael (ed.). The Focal Encyclopedia of Photography (4th ed.). Oxford, UK: Focal Press. pp. 28 et. seq. ISBN 978-0-240-80740-9.
- Lynne, Warren (2006). The Encyclopedia of 20th Century Photography. Routledge. pp. 515–520. ISBN 978-1-57958-393-4.
- "The Harvard College Observatory Astronomical Plate Stacks". SMITHSONIAN ASTROPHYSICAL OBSERVATORY. Archived from the original on 22 December 2015. Retrieved 16 December 2015.
- "Scientific Products". Ilford Photo. Archived from the original on 5 December 2015. Retrieved 16 December 2015.
- "1878-1929". Eastman Kodak. 2015. Archived from the original on 23 August 2015. Retrieved 8 August 2015.
- Hannavy John (2013). Encyclopedia of Nineteenth-Century Photography. Routledge. p. 251.
- "1878-1929". Eastman Kodak. Archived from the original on 2012-02-10. Retrieved 2016-01-01.
- "www.loc.gov". loc.gov. 2014. Archived from the original on 19 September 2015. Retrieved 8 August 2015.
- Day Lance McNeil Ian (2002). Biographical Dictionary of the History of Technology. Routledge. p. 631. ISBN 1-134-65020-5.
- Jacobson 2000, p. 266.
- "History of the digital camera and digital imaging". The Digital Camera Museum. Retrieved 10 August 2015.(section "1988/1989 – First Consumer Digital Cameras")
- "H&D curve of film vs digital". Archived from the original on September 23, 2015. Retrieved August 11, 2015.
- Claire Elise Campton (17 August 2016). "Film Photography". Photopholio. Archived from the original on 19 September 2016. Retrieved 17 August 2016.
- "This Is Why Film Photography Is Making a Comeback". Archived from the original on 2017-05-19. Retrieved 2017-10-28.
- "Archived copy". Archived from the original on 2017-07-08. Retrieved 2017-10-28.CS1 maint: archived copy as title (link)
- "Kodak Ektachrome E100 Film is Now Available in 120 and 4x5 Formats". petapixel.com. Retrieved 2020-06-03.
- "Archived copy". Archived from the original on 2017-10-29. Retrieved 2017-10-28.CS1 maint: archived copy as title (link)
- "Fotokemika Ceases Production, Affects Efke/ADOX". La Vida Leica!. Archived from the original on 2016-03-04. Retrieved 2016-01-01.
- Jacobson, Ralph E. (2000). The Focal Manual of Photography: Photographic and Digital Imaging (9th ed.). Boston, Mass.: Focal Press. ISBN 978-0-240-51574-8.CS1 maint: ref=harv (link)
|Wikimedia Commons has media related to Photographic films.|